Poly (µ-caprolactone) Fiber: An (9) P. (µ-caprolactone) Fiber: An Overview . Bahareh...
Embed Size (px)
Transcript of Poly (µ-caprolactone) Fiber: An (9) P. (µ-caprolactone) Fiber: An Overview . Bahareh...
Journal of Engineered Fibers and Fabrics 74 http://www.jeffjournal.org Volume 9, Issue 3 2014
Poly (-caprolactone) Fiber: An Overview
Bahareh Azimi1, Parviz Nourpanah1, Mohammad Rabiee2, Shahram Arbab3
1Amirkabir University of Technology, Textile Engineering Department, Tehran, IRAN
2Amirkabir University of Technology, Biomedical Engineering Department, Tehran, IRAN
3ATMT Research Institute, Faculty of Textile Engineering, Amirkabir University of Technology, Tehran, IRAN
Correspondence to: Parviz Nourpanah email: firstname.lastname@example.org
ABSTRACT Poly (-caprolactone), (PCL) or simply polycaprolactone as it is usually referred to, is a synthetic biodegradable aliphatic polyester which has attracted considerable attention in recent years, notably in the biomedical areas of controlled-release drug delivery systems, absorbable surgical sutures, nerve guides, and three-dimensional (3-D) scaffolds, for use in tissue engineering. Various polymeric devices like microspheres, microcapsules, nanoparticles, pellets, implants, and films have been fabricated using this polymer. It can be transformed by spinning into filaments for subsequent fabrication of desirable textile structures. Spinning may be accomplished by various approaches. The fibers may be fabricated into various forms and can be used for implants and other surgical applications such as sutures. Although numerous studies have investigated different properties and applications of PCL, there is no comprehensive study investigating different fabrication methods of PCL fibers and their biomedical applications. The present article presents a review on the production of PCL fiber via various methods, along with correlations between structure and properties of the fibers. The applications of these fibers in biomedical domains are also discussed. Keywords: PCL, Fiber, Spinning, Medical application. INTRODUCTION In recent years, biodegradable polymers have attracted considerable attention as biomaterials in pharmaceutical, medical, and biomedical engineering applications, including drug delivery systems, artificial implants, and functional materials in tissue engineering. Aliphatic polyesters, due to their favorable features of biodegradability and biocompatibility, comprise one of the most important classes of synthetic biodegradable polymers. The advantage of these polyesters is their biocompatibility and higher hydrolysability in the human body .
Poly (-caprolactone) (PCL) is a family member of biodegradable aliphatic polyesters which have found important use as biomaterials in prosthetics, sutures, and drug delivery systems. As a commercial material, the main attractions of PCL are (1) its approval by the Food and Drug Administration (FDA) for use in humans, (2) its biodegradability, (3) its compatibility with a wide range of other polymers, (4) its good processibility which enables fabrication of a variety of structures and forms, (5) its ease of melt processing due to its high thermal stability and (6) its relatively low cost [2-3]. It can also be transformed by spinning into filaments for subsequent fabrication of desirable textile structures. Due to excellent characteristics, such as biodegradability, biocompatibility, mild undesirable host reactions, and three-dimensional and directional porous structures, PCL fiber, whose diameter range from nanometer to millimeter, is broadly studied. In fiber form, PCL and its copolymers have been investigated for usage in drug delivery systems , long-lasting absorbable sutures [5-8] and, 3-D scaffolds for tissue engineering applications . For example, to use in absorbable nerve guides, -caprolactone has been copolymerized with DL-lactide  and trimethylene carbonate . PCL has received relatively comprehensive attention in the literature [3, 12-13], however, there are few studies investigating different fabrication methods and biomedical application of PCL fibers. The present article presents a review on the chemistry and different properties of PCL, production of PCL fiber by various methods and correlations between structure and properties of the fibers. The applications of these fibers in biological and medical domains are also discussed. Synthesis and Physicochemical Properties of PCL PCL is prepared by the ring opening polymerisation of the cyclic monomer -caprolactone (Figure 1) and was studied as early as the 1930s . Recently a
Journal of Engineered Fibers and Fabrics 75 http://www.jeffjournal.org Volume 9, Issue 3 2014
wide range of catalysts for the ring opening polymerization of caprolactone has been reviewed .
FIGURE 1. Ring opening polymerization of -caprolactone to polycaprolactone. Catalysts such as stannous octoate are used to catalyze the polymerization and low molecular weight alcohols can be used to control the molecular weight of the polymer . There are various mechanisms which affect the polymerization of PCL and these are anionic, cationic, co-ordination and radical. Each method affects the resulting molecular weight, molecular weight distribution, end group composition and chemical structure of the copolymers . The number average molecular weight of PCL samples generally vary from 3,000 to 80,000 g/mol and can be graded according to the molecular weight . It is a semi-crystalline polymer with a melting point of 5964 C and a glass-transition temperature of 60C . PCL is soluble in chloroform, dichloromethane, carbon tetrachloride, benzene, toluene, cyclohexanone and 2-nitropropane at room temperature. It has a low solubility in acetone, 2-butanone, ethyl acetate, dimethylformamide and acetonitrile and is insoluble in alcohol, petroleum ether and diethyl ether . The versatility of PCL is due to the fact that, it allows modification of its physical, chemical and mechanical properties by co-polymerization or blending with many other polymers efficiently. It has been observed that co-polymerization alters the chemical property that indirectly affects all other properties such as crystallinity, solubility, and degradation pattern resulting in a modified polymer with intended properties for drug delivery . Whereas, blending that leads to altered physical property and biodegradation along with highly influenced mechanical properties is preferred for formulations of tissue engineering such as scaffolds, fibers and films. A number of polymers have been studied for their compatibility to modify the thermal, rheological as well as biophysical properties of PCL, based on its application. PCL is reported to be compatible with natural polymers like starch, hydroxy apatite (HA), chitosan and synthetic polymers namely
poly ethylene glycol (PEG), poly urethane (PU), oxazolines, poly ethylene oxide (PEO), poly vinyl alcohol (PVA), polylactic acid and polylactic co-glycolic acid (PLGA) [19-26]. These PCL modifications satisfy the required biophysical properties for most of the formulation currently used in drug delivery . Biodegradation PCL is degraded by hydrolysis of its ester linkages in physiological conditions (such as in the human body) and has therefore received a great deal of attention in order to be used as an implantable biomaterial. In particular it is especially interesting for the preparation of long term implantable devices, due to its degradation which is even slower than that of polylactide. From degradation studies presented in the literature it can be concluded that PCL undergoes a two-stage degradation process: firstly the non-enzymatic hydrolytic cleavage of ester groups and secondly, when the polymer is more highly crystalline and has a low molecular weight (less than 3000) the polymer is shown to undergo intracellular degradation as this was observed during experiments of PCL fragments uptake in phagosomes of macrophages and giant cells and within fibroblasts . This supports the theory that PCL may be completely resorbed and degraded via an intracellular mechanism once the molecular weight was reduced to 3000 or less. It was also noted that in the first stage the degradation rate of PCL is essentially identical to the in vitro hydrolysis at 40C and obeyed first-order kinetics. It was concluded that the mechanism of PCL degradation could be attributed to random hydrolytic chain scission of the ester linkages, which caused a decrease in molecular weight. The homopolymer PCL has a total degradation of two to four years (depending of the starting molecular weight of the device or implant) [28-29]. The rate of hydrolysis can be altered by copolymerization with other lactones or glycolides/lactides. Surprisingly, more than 1000 papers have been published during the last decade in the biomaterials and tissue engineering literatures which use PCL-based-scaffolds. Among these studies only a small number of groups have included a study of the degradation and resorption kinetics of the PCL scaffolds . Table I shows comprehensive data on PCL fiber degradation. Spinning of PCL Fibers As mentioned previously, PCL by itself is most suited biomedically to the design of long-term implantable systems. In fiber form, PCL has also been investigated for use in drug delivery systems, long-lasting absorbable sutures and, most recently,
Journal of Engineered Fibers and Fabrics 76 http://www.jeffjournal.org Volume 9, Issue 3 2014
3-D scaffolds for tissue engineering applications. Extrusion of the PCL into monofilament and multifilament may be achieved by fiber formation
mechanisms such as melt spinning, solution spinning, and electrospinning. There are distinct features of each of these processes that are subsequently reflected